Presentation on theme: "Abrasive Processes Abrasive machining involves material removal by the action of hard abrasive particles that are usually in the form of a bonded wheel."— Presentation transcript:
1Abrasive ProcessesAbrasive machining involves material removal by the action of hard abrasive particles that are usually in the form of a bonded wheel.These operations are generally used as finishing operations, although in some cases they are used for high metal removing rates rivaling of conventional machining operations.These processes include grinding, honing, lapping, super finishing, polishing and buffing.
2Surface roughness (Ra) in μm ProcessPart GeometrySurface roughness (Ra) in μmGrindingFlat, External cylinder0.406 – 1.60.203 – 0.406HoningRound hole0.102 – 0.813LappingFlat or slightly spherical– 0.406Super finishing– 0.203PolishingDifferent shapes.– 0.813buffing– 0.406
3The reasons for the commercial and technological importance of the abrasive processes are; They can be used on all types of materials, ranging from soft to hard materials.Some of theses processes can produce extremely fine surface finish. (see the previous table).The dimension of the product can be held to extremely close tolerances.
4Grindingit is a material removal processes in which the abrasive particles are contained in a bonded grinding wheel that operates at very high surface speeds.The grinding operation is much like the milling operations. Cutting occurs either the periphery or the face of the grinding wheel, similar to the peripheral milling and face milling. The peripheral grinding is much common than the face one.Grinding wheelGrinding wheel
5The difference between the milling operations and the grinding operations are; The cutting edgesDefined number of cutting edges (teeth)The abrasive is smaller and more numerous (undefined number of grains).Cutting speedMuch higherCutting anglesDefined cutting anglesRandomly oriented and can possess very high negative rake anglesReshaping of the cutting edgesThe dull abrasive particles either fracture to create a fresh cutting edges or pulled out to expose a new grains.
6Grinding wheelThe grinding wheel is the tool with which the grinding action is performed.It consists of abrasive particles and bonding materials, (as shown in the Fig.).The bonding material holds the particles in place and build the shape and structure of the wheel.These two components and the way they are fabricated determine the parameters of the grinding wheel;Abrasive materials Grain size3. Bonding materials. 4. Wheel grade5. Wheel structure
71- Abrasive materials General properties of abrasive materials are; High hardnessWear resistanceToughnessFriability; it is the ability of the abrasive material to fracture, when the cutting of the grain becomes dull, thereby exposing a new cutting edge (sharp cutting edge).
8Steel, other ferrous materials and high strength alloys. Abrasive materialsMarkingUsingAluminum Oxide (Al2O3)ASteel, other ferrous materials and high strength alloys.Silicon carbide (SiC)CDuctile metals (AL, brass, and stainless steel), and brittle materials (CI, and certain ceramics).Cubic born nitride (CBN)BHard materials (hardened tool steels and aero space alloys).DiamondDHard abrasive materials (ceramics, cemented carbides and glass).
92- Grain sizeIt’s an important parameter in determining the surface finish and metal removing rate.Grain size surface finishGrain size material removal rate .Harder work materials required smaller grain size while the softer materials required larger grit size. Grit size is measured using a screen mesh. Smaller grit size has larger numbers.The selection of the grit size must take into consideration the above 3 points.
103- Bonding materialsThe bonding material holds the particles in place and build the shape and structure of the wheel.The desirable properties of bonding materials are;Strength (withstand centrifugal forces).Toughness (resist shattering in shock loads).Hardness.Temperature resistance (withstand high temperature).Hold abrasive material in place rigidly to accomplish the cutting forces while allowing the grain that are worn to be dislodged so that new grains can be exposed.
11most fixable, used in cut-off wheels. Resinoid bond B Bonding materialsMarkingUsingVitrified bondVStrong, rigid, resist temp., relatively unaffected by water and oil that used in grinding fluids.Silicate bondSLimited to situations in which heat generated must be minimized.Rubber bondRmost fixable, used in cut-off wheels.Resinoid bondBVery high strength, used for rough grinding and cut-off operations.Shellac bondEStrong but not rigid, for good finish.Metallic bondMCommon for diamond and cubic born nitride, usually bronze.
12Vb bond materials proportion Vp voids (pores) proportion 4- Wheel StructureRefers to the relative spacing of the abrasive grains in the wheel.It is measured on a scale ranges from open to dense (the ratio between the grains proportion to bond materials proportion).Open is used for chip clearance.Dense one is used for surface finish and dimensional control.Vg + Vb + Vp = 1.0Vg grains proportionVb bond materials proportionVp voids (pores) proportion
13Wheel GradeIndicates the wheel’s bond strength in retaining the abrasive grits during cutting. Dependent on the present of bonding materials (Vb).It is measured on a scale ranges from soft to hard.Soft one, lose the grains readily, is used for low materials removal rates and when machining hard work material.Hard one, retains the grains, is used for high materials removal rates and when machining soft work material.
18There are two types of feed; Cross feed; motion of work table (w) In feed; the motion of the wheel into the work (d)- In the cutting, parameters and the grinding wheel parameters have a direct effect into;1- Surface finish2- Forces and energy3- Temperature of the work surface4- Wheel wear5- Machining time.
19Surface finish Number of chips formed; C is grits/mm2 (from 0.1 to 10) It is affected by the size of the individual chips (note that small grit size get better surface finish).Number of chips formed;C is grits/mm2 (from 0.1 to 10)That mean that the increase of V and C for a given w increase the number of chips/time and improve the finish.
20U specific energy, Fc cutting force. Forces and energyU specific energy, Fc cutting force.Specific energy in the grinding operations is much greater that in other conventional machining because;The size effect in the machining.High negative rake angle of the individual grains.Not all the grits are engaged in actual cutting (cutting, plowing, and rubbing, Fig. 8.5).Example 8.1 page 193
21Temperatures at the work surface The grinding process generates high temperature because the size effect and the high negative rake angle, this with high friction.This high temperature can have several damaging effects;Bums and cracks;Bum is a discolorration on the surfaceCracks are perpendicular to the wheel speed directionSoftening of the work surface.Residual stresses.The proper application of the cutting fluids reduce friction and remove heat and washing away chips.
22Wheel wearIn the grinding wheel there are three types of wear (Fig. 8.6);Grain fracture, 1st region.Attritions wear, 2nd region.Bond fracture, 3rd region.When the wheel in the 3rd region, it should be re-sharping (dressing operation) to;Breaking off dulled grits.Removing the chips.Grinding ratio (GR) is between 95 to 125, depending on wheel speed which reduce the wear, while at too high speed both wear and temp. are increased and the grinding ratio is reduced with the surface finish.
23Machining timeB work widthb grinding wheel widthl work lengthΔ allowance (≈10mm)h total depthd infeedVw the work speedw cross feedExample 8.2 page 199
24Grinding operations 1- Surface Grinding Used to finish products created with other operations.Shapes to be grinded are plain surfaces, internal and external cylinders, and contour surfaces.The contour surfaces, such as thread, are created by a special formed wheels, which are created in the tool rooms.1- Surface GrindingPerformed using either the periphery or the flat surface of the grinding wheel (face grinding).The peripheral grinding is performed with a horizontal axis machines, while the face grinding is performed with a vertical axis machines, as shown in the figure.
25Note the direction of the cross feed and in-feed Horizontal spindle with reciprocating worktable.Horizontal spindle with rotary worktable.vertical spindle with reciprocating worktable.Vertical spindle with rotary worktable.Note the direction of the cross feed and in-feed
262- cylindrical Grinding a- External cylindrical grindingthe feed motions are either traverse feed (the wheel or workpiece or both) or plunge cut.b- Internal cylindrical grinding
27External Centerless Grinding The workpiece is not held between center, then it used for high production rate machining, no holding time.The regulating wheel rotates at lower speed and is inclined at a slight angle I, the feed rate of this wheel depending on its diameter, rotating speed, and its angle.External Centerless Grinding
28The internal centerless grinding has two supporting rolls instead of the rest blade in the external one.Internal Centerless Grinding
294- Creep Feed GrindingdFeedIn-Feed are 1000 to times greater then conventional oneFeed rates are reduced about the same proportion.High MRR and productivity because of the continuous cutting.Advantages;High MRRImprove accuracyReduced temperatures.
30Related abrasive processes 1- HoningTo finish the bores of internal combustion engines, bearing, hydraulic cylinders, and gun barrels.Performed with a set of bonded abrasive sticks.Its motion is combination of rotation and linear motion.Speed between 15 to 150 m/min.Grit size between 30 and 600ToolOperation
312- LappingUsed to produce surface finish of extreme accuracy and smoothness.Used in production of optical lenses, metallic bearing surface, and gages.It used a fluid suspension of very small abrasive particles (in oils or kerosene) between the work and the lapping tool.Common abrasives are aluminum oxide and silicon carbide with grit size between 300 and 600.The tool takes the inverse shape of the work part.Materials such as steel, CI, copper, lead and wood.
323- Superfinishing Like honing but; Shorter strokes Higher frequancy, lower pressureLower workpiece speed.Smaller grit size.Only one stick is used
334- Polishing and Buffing Polishing is used to remove scratches and burrs and smooth rough surfaces by means of abrasive grains attached to the polishing wheel rotating at high speed around 2250 m/min.The wheel, flexible wheel, is made of leather, canvas, felt and papers. And grit size of 20 to 80 for rough, 90 to 120 for finish.Buffing is similar to polishing with softer wheels, finer abrasive materials.Speed ranging from 2400 to 5100 m/min.